Flux Synthesis, Crystal Structures, and Physical Properties of New Lanthanum Vanadium Oxyselenides
Peschke, Simon; Gamperl, Lisa; Weippert, Valentin; Johrendt, Dirk; Dalton Trans.  (2017) –; doi:10.1039/C7DT00779E

data_7042688
_publ_section_title
;
 Flux Synthesis, Crystal Structures, and Physical Properties of New
 Lanthanum Vanadium Oxyselenides
;
_journal_name_full               'Dalton Trans.'
_journal_paper_doi               10.1039/C7DT00779E
_journal_year                    2017
_chemical_compound_source        'see text'
_chemical_formula_moiety         'La5 O5 Se7 V3'
_chemical_formula_sum            'La5 O5 Se7 V3'
_chemical_formula_weight         1480.09
_chemical_name_common            lanthanum_vanadium_selenide_oxide
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   ' .'
_atom_sites_solution_primary     ' ?'
_atom_sites_solution_secondary   ' ?'
_audit_update_record
;
2017-03-02 deposited with the CCDC.
2017-03-31 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.5036(2)
_cell_length_b                   3.9012(7)
_cell_length_c                   24.757(1)
_cell_measurement_reflns_used    9904
_cell_measurement_temperature    293
_cell_measurement_theta_max      35.00
_cell_measurement_theta_min      2.60
_cell_volume                     1594.0(3)
_computing_publication_material  'PLATON (Spek, 2003)'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0623
_diffrn_reflns_av_sigmaI/netI    0.0354
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_limit_l_min       -39
_diffrn_reflns_number            41381
_diffrn_reflns_reduction_process
;
;
_diffrn_reflns_theta_full        35.08
_diffrn_reflns_theta_max         35.08
_diffrn_reflns_theta_min         2.47
_exptl_absorpt_coefficient_mu    30.748
_exptl_absorpt_correction_T_max  0.7469
_exptl_absorpt_correction_T_min  0.5032
_exptl_absorpt_correction_type   numerical
_exptl_crystal_density_diffrn    6.168
_exptl_crystal_density_method    'Not Measured'
_exptl_crystal_F_000             2528
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.01
_exptl_crystal_size_min          0.01
_refine_diff_density_max         2.880
_refine_diff_density_min         -2.840
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.030
_refine_ls_hydrogen_treatment    ' .'
_refine_ls_number_parameters     121
_refine_ls_number_reflns         3959
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0454
_refine_ls_R_factor_gt           0.0237
_refine_ls_shift/su_max          0.038
_refine_ls_shift/su_mean         0.006
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     W=1/(\S^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0421
_refine_ls_wR_factor_ref         0.0472
_reflns_number_gt                2958
_reflns_number_total             3959
_reflns_threshold_expression     i>3\s(i)
_cod_data_source_file            c7dt00779e2.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_database_code               7042688